Discussion Chain ID: 42755
================================================================================

User asked: Why did I get these inconsistent experimental results in silanization?

I used a 50% wt mixture of Tetraethylorthosilicate + Kerosene for silanization of some glass plates with **different treatment times** (from 1 sec to 35 sec). However, the contact angle(CA) that I got does not seem consistent as it does not always increase as I increase the treatment time (when treatment time increases, the CA fluctuates). What might be the reason? and whether I should change the method or the solution(s)? P.S. I cleaned the glass with acetone in a sonicator. Then I put the glass into solution and after specific time put it into water to clean the solution from surface and then clean the remaining oil (from kerosene) by rubbing a napkin to the glass plate. Then I measured the CA.

Answer 1 (3 votes):
Rubbing is a very inconsistent process, and will introduce a lot of variation. I would suggest using a volatile non-polar solvent such as acetone, hexanes, or ethyl acetate to remove residual kerosene and allowing to air dry.

Discussion on this answer:
Comment: So, do you mean the main issue that may cause this fluctuations in CA could be this rubbing that I've done with a napkin?(I mean do you think that if I perform the process correctly, I should basically get the lowest CA in 1 sec treatment and the highest CA in 35 sec. Is that right?)
Comment: In theory there should be a correlation, but tetraethoxysilane (TEOS) is not a good chemical for silanization, as the ethoxy group can easily hydrate leaving you with a hydrophilic $\ce{Si}-\ce{O}-\ce{H}$ surface. I did assume everything else you did was the same, but factors such as humidity and exposure time to air can affect results due the the nature of TEOS
Comment: I have the following three more solutions available. Based on your above comment that TEOS is not very appropriate for silanization, do you think which solution is the more suitable one for creating different levels of hydrophobicity? (please also let me know if there are any instructions for silanizing that you think I should know) 1) ChloroTrimethylSilan 2) OctaDecylTrichloroSilan 3) DichloroDimethylSilan
Comment: I like chlorotrimethylsilane because it has only one chloro group, and octadecyltrichlorosilane because it is sterically bulky. The latter should work best from the steric, but the former gives complete surface reaction, so I cannot say with certainty.
Comment: One other thing to consider. Are you using a consistent amount of water? This can affect your contact angle.
Comment: I'm not sure what you mean by "using water" as I use water only for cleaning purposes. Could you please explain it?
Comment: What material are you using for contact angle measurements?
Comment: Oh, I see what you mean. Yes, I don't change the water drop volume in all my CA measurements.
Comment: I need one CA less than 90 as well and I realized that when I use kerosene in my silan solution, it is hardly cleaned from glass surface. Since each coated particle is only one time in contact to water (and the coating cannot be easily washed), do you think I can use only kerosene as a coating to give a ~60 deg CA to my glass particle that I want to launch them to my water droplets? OR it may not give a consistent CA.


================================================================================

